Lecture # 3. Civil Engineering Material Fine and Coarse aggregates Dr. Attaullah Shah . Department of Civil Engineering Swedish College of Engineering and Technology-Wah Cantt. . Aggregates:. Aggregates make up 60-75% of total volume of concrete.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Civil Engineering Material
Fine and Coarse aggregates
Dr. Attaullah Shah
Department of Civil Engineering
Swedish College of Engineering and Technology-Wah Cantt.
Smallest sieve opening through which the entire amount is required to pass.
Nominal Max. size:
Largest sieve opening through which a specified quantity may be retained
Aggregate that has a particle size distribution such that, when compacted, the voids (as a % of volume) are relatively small.
Aggregate that has a particle size distribution such that, when compacted, the voids (as a % of volume) are relatively large.
Igneous (solidification of molten material
Sedimentary (consolidated transported material)
Metamorphic (preexisting rock changed by temperature or pressure over time)
Material that covers the bedrock which may be cm or km in thickness
Boulders, cobbles, gravel, sand, silt, clay
React with Acids
Luster (dull, glassy)
Group I –Glassy
Group II – Dull, Fine Grain
Scratch with a knife
Hard - Chert, Basalt
Group III - Granular
Scratch with a knife
Silica and Silicates
hard, strong, insoluble
hydrous silicate (3-9%)
hard, strong, variable composition
softer, strength variable
1CaCO3 + 1MgCO3
softer, strength variable
excellent strength and hardness
avoid contamination with silts, shale and clay
variable strength and durability with porosity, absorption
dense strong aggregate
many types are reactive with alkalies
Limestone + Dolomite
Lower modulus than silicates (softer)
porosity and absorption vary considerably
good aggregate source
Size (maximum, distribution)
Texture (smooth, porous)
Freeze thaw stability
Integrity during heating
(unit mass or bulk density)
Normal-weight concrete… bulk density of aggregate is approximately 75-110 lb per cubic foot.
• Void content affects mortar requirements in mix design; water and mortar requirement tend to increase as aggregate void content increases.
• Void content between aggregate particles increases with increasing aggregate angularity.
• Void contents range from 30-45% for coarse aggregates to about 40-50% for fine aggregates.
• Total volume of voids can be reduced by using a collection of aggregate sizes.
The cement paste requirement for concrete is proportional to the void content of the combined aggregate.
Specific Gravity (Relative density)
Absolute:the ratio of the weight of the solid to the weight of an equal volume of water (both at a stated temperature)
- Refers to volume of the material excluding all pores
Apparent:ratio of the weight of the aggregate (dried in an oven at 212- 230ºF for 24 hours) to the weight of water occupying volume equal to that of the solid including the impermeable pores
- Volume of solid includes impermeable pores (but not capillary pores)
Used for calculating yield of concrete or the quantity of aggregate required for a given volume of concrete.
Particle Shape and Surface Texture
• Rough textured, angular, elongated particles require more water to produce workable concrete than do smooth, rounded, compact aggregates.
• Aggregates should be relatively free of flat and elongated particles (limit to 15% by weight of total aggregate).
• Important for coarse and crushed fine aggregate - these require an increase in mixing water and may affect the strength of the concrete, if cement water ratio is not maintained.
Shrinkage of Aggregates:
fine grained sandstones, slate, basalt, trap rock, clay-containing
Large Shrinkage =
Low Shrinkage =
quartz, limestone, granite, feldspar
What happens if abnormal aggregate
• Excessive cracking
• Large deflection of reinforced beams and slabs
• Some spalling (chipping or crumbling)
If more than 0.08 percent shrinkage occurs, the aggregate is considered undesirable.
Absorption and Surface Moisture
If water content of the concrete mixture is not kept constant, the compressive strength, workability, and other properties will vary from batch to batch.
D 4791 Elongation test
Moisture Conditions of Aggregates:
1.Oven dry- fully absorbent
2. Air dry- dry at the particle surface but containing some interior moisture
3. Saturated surface dry (SSD) –neither absorbing water nor contributing water to the concrete mixture.
4. Wet or moist- containing an excess of moisture on the surface
Absorption Capacity: maximum amount of water aggregate can absorb
• Absorption Capacity (%) = [(WSSD – WOD)/WOD] X 100
Surface Moisture: water on surface of aggregate particles
• Surface Moisture (%) = [(WWET – WSSD)/WSSD] X 100
Moisture Content: of an aggregate in any state
•Moisture Content (%) = [(WAGG – WOD)/WOD] X 100
Abs. = (WSSD - WOD) / WOD x 100%
Reactivity to alkalies
Reactivity to CO2
Na or Mg sulfate saturated solutions are used to test aggregate friability
5 cycles of saturation and drying
Sulfates hydrate and expand to fracture weak planes
Loss is determined by mass
12% max loss w/ Na
18% max loss w/ Mg
Precision is very poor
Typical results of losses between 10 and 40%.
40% is the max. limit
Coefficient of Variation
Single Operator – 2%
Multilab – 4.5%
Two tests by the same operator on the same sample should not vary by more than 2.83*2.0=5.7% on the % loss (the 2.83 represents 1 in 20 samples outside the range coefficient).